Home >
Documents >
POLITECNICO DI MILANO · 2014-11-28 · POLITECNICO DI MILANO Dipartimento di Chimica, Materiali e...

Share this document with a friend

Embed Size (px)

of 94
/94

Transcript

POLITECNICO DI MILANO

Dipartimento di Chimica, Materiali e Ingegneria Chimica

“Giulio Natta”

Scuola di Ingegneria Industriale e dell’Informazione

SHEAR STABILITY OF POLYMERIC

COLLOIDAL DISPERSIONS:

INTERPLAY BETWEEN AGGREGATION AND COALESCENCE

Relatore: Prof. Davide Moscatelli

Correlatore: Dr. Miroslav Soos

Autore:

Luca Colonna

Matr. n. 797553

Anno Accademico 2013-2014

2

Contents

Acknowledgments ...................................................................................................... 4

Abstract ...................................................................................................................... 5

1 INTRODUCTION............................................................................................... 6

1.1 Emulsion Polymerization: .............................................................................. 6

1.1.1 Description of the process: .................................................................. 6

1.1.2 Composition and size control ............................................................... 9

1.2 Stability of colloidal suspensions: ................................................................ 11

1.3 Interaction between colloid particles: ........................................................... 13

1.3.1 Attractive interactions: ....................................................................... 13

1.3.2 Repulsive interactions: ....................................................................... 13

1.3.3 DLVO theory ...................................................................................... 15

1.4 Aggregation ................................................................................................. 18

1.4.1 Diffusion limited cluster aggregation kernel ....................................... 19

1.4.2 Reaction limited cluster aggregation kernel ....................................... 21

1.4.3 Shear induced aggregation kernel ..................................................... 24

1.5 Gelation ....................................................................................................... 26

1.6 Coalescence ................................................................................................ 27

2 SAMPLES PREPARATION: ........................................................................... 28

2.1 Synthesis: .................................................................................................... 28

2.1.1 Materials: ........................................................................................... 28

2.1.2 Equipment: ........................................................................................ 30

2.1.3 Protocol: ............................................................................................ 30

2.2 Purification: .................................................................................................. 31

2.2.1 Materials: ........................................................................................... 31

2.2.2 Protocol: ............................................................................................ 32

2.3 Composition control: .................................................................................... 33

2.3.1 Equipment: Differential scanning calorimetry ..................................... 33

2.3.2 Protocol: ............................................................................................ 33

3 SAMPLES CHARACTERIZATION: ................................................................. 35

3.1 Light scattering ............................................................................................ 35

3.1.1 Static light scattering theory: .............................................................. 35

3.1.2 Protocol: ............................................................................................ 37

3

3.1.3 Dynamic light scattering theory: ......................................................... 38

3.2 Titration ....................................................................................................... 39

3.2.1 Theory: .............................................................................................. 39

3.2.2 Protocol: ............................................................................................ 40

3.3 ζ-potential .................................................................................................... 40

3.3.1 Theory: .............................................................................................. 40

3.3.2 Protocol: ............................................................................................ 42

3.4 Rheometer ................................................................................................... 43

3.4.1 Theory: .............................................................................................. 43

3.4.2 Protocol: ............................................................................................ 44

4 RESULTS AND DISCUSSION ........................................................................ 45

4.1 Stagnant Aggregation .................................................................................. 46

4.1.1 DLCA: ................................................................................................ 46

4.1.2 RLCA ................................................................................................. 58

4.2 Shear Aggregation ....................................................................................... 63

4.2.1 Salt effect ........................................................................................... 70

4.2.2 Temperature effect ............................................................................ 71

4.2.3 Composition effect ............................................................................. 76

5 CONCLUSION: ............................................................................................... 79

References ............................................................................................................... 82

APPENDIX I ............................................................................................................. 84

APPENDIX II ............................................................................................................ 86

APPENDIX III ........................................................................................................... 92

4

Acknowledgments

I want to express my deep gratitude to Professor Morbidelli for introducing me to the

wonderful world of colloids and for giving me the opportunity to develop my master

thesis in his research group at the ETH Zurich. I am very thankful to Professor

Moscatelli, Dr. Soos, Dr. Bastian Brand, Baptiste Jaquet and Dr. Stefano Lazzari for

their valuable supervision, outstanding patience, lesson and help.

In primis vorrei ringraziare di tutto cuore i miei genitori Ezio e Silvia per i valori che mi

hanno trasmesso e per tutti i sacrifici fatti per permettermi di arrivare dove sono.

Molte altre persone hanno reso possibile questo lavoro di tesi con il sostegno e

l’appoggio che mi hanno sempre dimostrato, in particolare voglio ringraziare mia

nonna Anna, la mia fidanzata Stefania, le mie sorelle Lucia e Cecilia, la zia Federica,

i carissimi amici Alessio, Alessio, Christian, Francesco, Giovanna, Giulia, Marcello,

Riccardo e Tommaso.

Ganz besonders möchte ich mich bei Steffi und Peter Lüthy dafür bedanken, dass sie

mich in ihrer Familie so herzlich aufgenommen haben und mir in schwierigen

Momenten mit Rat und Tat zur Seite standen.

Alla memoria della mia cara nonna Giovanna

5

Abstract

The aim of the present work is to study the role that coalescence plays in the

aggregation under shear of polymeric colloidal dispersions.

Understanding the role of coalescence is very important not only from the scientific

point of view, since at the moment in the literature a unified depiction of this

phenomenon is missing, but also from the industrial one: indeed, coalescence is

involved in many applications concerning the manufacture of polymer colloidal

products and the design of polymer processes.

In the present study four samples of poly(methyl methacrylate –co- butyl acrylate)

latexes have been synthesized by starved emulsion polymerization in a semi-batch

reactor. Changing the monomer ratios leads to polymer particles exhibiting a glass

transition temperature gradient which allows studying the coalescence process.

The coalescence behavior of our systems has been first clarified in stagnant

conditions; while in a second stage shear conditions have been investigated.

6

1 INTRODUCTION

1.1 Emulsion Polymerization:

1.1.1 Description of the process:

Emulsion polymerization is a very common process in industrial application. It allows

the production of a colloidal dispersion of polymer nanoparticles with a diameter of

50-500 nm in a continuous medium called latex and is typically carried out in stirred-

tank reactors, which usually operate in a semi-continuous mode, although both batch

and continuous operations are also used.

If the continuous phase is water one speaks of direct emulsions, otherwise of inverse

emulsions. A typical direct emulsion polymerization process involves: monomers,

water, surfactant and a water soluble initiator.

In a batch emulsion polymerization, at the beginning of the process the mixture of

monomers is dispersed in water by stirring. Monomer droplets (100-1000µm) are

formed and then stabilized by the emulsifier adsorbed on their surface.

The available surfactant actually partitions between the surface of the monomer

droplets and the aqueous phase; if both the monomer droplets and the aqueous

phase are saturated and further surfactant is added, the formation of micelles occurs.

The concentration at which these aggregates are formed is the so called critical

micellar concentration (CMC) (cf. Figure 1-1).

Figure 1-1 Trends of surface tension [J/m2] and emulsif ier concentration [mol/m

3] as a

function of the added amount of emulsif ier per uni t volume [mol/m3]: once the

dispersion is saturated (cmc), since micelles are forming, the surface tension/emulsif ier

concentration stop decreasing/ increasing and remain constant. Picture taken from [1]

7

Polymerization starts after the addition of water-soluble initiators. When a water-

soluble initiator is added to the monomer dispersion, radicals are formed. They are

usually too hydrophilic to enter the organic phase and rather react with the monomer

dissolved in the aqueous phase, forming oligoradicals; after adding few monomer

units they become quickly hydrophobic, giving rise to particle formation. In particular

depending on 0E , the initial amount of surfactant, two processes of polymer particle

formation (i.e. nucleation) are possible: heterogeneous nucleation and homogeneous

nucleation. In case of heterogeneous nucleation as 0E > CMC, micelles are present

and oligoradicals diffusive in the micelles, nucleating them. In case of homogeneous

nucleation 0E < CMC, there is not sufficient surfactant in order to form micelles; the

propagating radicals reach a critical length, become too hydrophobic and precipitate,

creating particles nuclei. The emulsifier present in the system will adsorb onto the

newly formed interface stabilizing the polymer particles. In both nucleation

mechanisms, the oligoradicals could diffuse also into the monomer droplets. This

further nucleation mechanism can be typically neglected, as the surface/volume ratio

of the micelles in the heterogeneous nucleation case is much larger than the one of

monomer droplets, being the latter three orders of magnitude larger in size.

Focusing on heterogeneous nucleation, as soon as the radicals enter the micelles,

polymer particles are formed. In principle, a radical can terminate in the aqueous

phase, enter previously formed particles or enter monomer droplets, but, if we

assume a fast nucleation, all radicals enter completely micelles; it is worth to point

out that radicals are formed during all the polymerization process, in fact their

characteristic time of formation is larger than the monomer addition one. After

typically 5-10% of conversion micelles are completely consumed by the entry of

radicals and the stabilization of growing particles. This is the end of the nucleation

and after that the number of particles will remain constant; this stage of the process is

called interval I (cf. Figure 1-2). In interval II the system is composed by monomer

droplets and monomer swollen polymer particles (up to 60% of their volume fraction),

growing in time due to radical entry. The monomer diffuses from the droplets through

the water on the polymer particles in order to maintain its volume fraction on particles

constant. This interval continues as long as monomer droplets are present. In interval

III monomer concentration in polymer particles and water phase decreases

continuously. The rate of polymerization decreases so until the end of the process.

8

An exhaustive mathematical formulation of the batch emulsion polymerization kinetic

mechanism can be found in [2].

Figure 1-2 Intervals in batch heterogeneous emulsion polymerization. Picture taken

from [3]

9

1.1.2 Composition and size control

In batch copolymerization processes it is important to control the chain composition

due to the so-called composition drift occurring the more the reacting monomers

exhibit different reactivity. To clarify this point, consider two monomers A and B,

where both A and B preferentially react with A rather than with B (A has a larger

reactivity ratio than B). Be 0

AX the molar fraction of monomer A at time zero, the

instantaneous chain composition of polymer AF contains a certain fraction of

monomer A, which is calculated via the Mayo-Lewis plot (cf. Figure 1-3). As the

reaction takes place, the monomer phase becomes poorer of A and AX decreases,

leading the subsequent polymer chains to be as well poorer in A in composition (i.e.

AF decreases, cf. arrow in Figure 1-3 )

This issue can be well appreciated looking at a general Mayo Lewis plot.

Figure 1-3 Mayo-Lewis plot in case the monomer A is the most reactive. Picture taken

from [1]

It is very clear that the composition drift strongly affects the average composition of

the chains. To avoid the composition drift, emulsion polymerization can be carried out

in semibatch reactors, where a proper flow rate of the two monomers is fed to keep

their mole fractions in the reactor constant.

The general mass balance for the ith-monomer species in a semibatch reactor is:

10

ii pi

dNN R V

dt (1.1)

Where iN , iN , piR and V represent the moles, the molar flow rate, the

polymerization rate of the ith-monomer and the reactor volume.

The reactor under consideration admits only one stable pseudo-steady state at

sufficiently large times, equation (1.1) simplifies to:

0idN

dt (1.2)

. pssa

i pi pi iN R V k R N (1.3)

Where .R is the overall concentration of radicals and pik . is the pseudo-propagation

rate constant of the ith-monomer species. The system evolves from the initial

monomer concentrations approaching the steady state ones.

It is so a self-regulated system and by only keeping the two flow rates of the

monomers at the value which grants the desired AF , we can achieve composition

control. Taking long feed times imposes to the system a much slower dynamics than

its intrinsic, which is the monomer consumption. From a physical point of view all the

monomer fed is immediately consumed as soon as it enters the system and

monomer droplets cannot be formed. This operation modus is referred to as starved.

In starved operations there is no monomer accumulation, and the global conversion

overlaps with the monomer feed. Size control can be easily achieved in starved

emulsion polymerization: as the particles grow progressively upon monomer addition,

it is sufficient to stop the feed as the required particle size is reached.

11

1.2 Stability of colloidal suspensions:

A system state is considered stable if it returns unchanged to its original condition,

after any perturbation that occurs. A process that evolves toward a stable state can

be more accurately described in terms of thermodynamic functions: if it tends to a

stable state, the variation of Gibbs free energy G of this process is negative.

For general dispersion processes (cf. Figure 1-4) the variation of the surface free

energy surfG is given by:

surfG A (1.4)

Figure 1-4 Dispersion process from a bulk to a dispersed state. Picture taken from [1]

is the surface tension at the interface and is twice the work per unit area required

to separate up to infinite two parts of a liquid column; it can be interpreted as the

work per unit area to create a new surface. A is the variation of the system specific

surface from the bulk (single big aggregate) to the dispersed state (colloid particles).

Since smaller particles have a larger area/volume ratio A is always positive.

The stability of such a system depends so on the sign of (cf. equation (1.4)): if the

surface tension is positive, the colloidal dispersion is unstable; in fact positive

means that positive work enters the system (i.e. stirring) in order to produce surfaces

and maintain clear interphases separation (without stirring the particles would tend to

collide, aggregate and return to their previous bulk state); on the other side if is

negative, the colloidal system is stable; the particles remain “well dispersed”

constituting a single phase with the dispersant medium.

In spite of thermodynamics, which states regardless time only the equilibrium state of

a system, a temporary concept of stability can be introduced: kinetic meta-stability.

12

A kinetic meta-stable state is not the final stable configuration of the system but only

a transient state in which the system remains for sufficient long times, slowly evolving

towards the thermodynamic one.

Due to their nanoscale nature colloidal particles undergo only Brownian motion: they

move randomly with an average kinetic energy proportional to Bk T and follow

Maxwell-Boltzmann speed distribution. This thermal agitation leads the particles to

collide with one another and then to aggregate. In order to limit the aggregation-worth

collisions an energy barrier sufficiently large to deal with the thermal energy can be

built. Introducing such an energetic barrier, which can be overcome only by few

particles according to Maxwell-Boltzmann speed distribution, increases the so called

system shelf-life and makes the system kinetically meta-stable.

In general colloidal systems depending on their stability can be classified as lyophilic

(stable) or lyophobic (unstable). Lyophobic colloids can be made kinetically meta-

stable by bringing charges on the particles surfaces or coating the particles with

some material that provides steric repulsion (cf. Figure 1-5).

Figure 1-5 Building an energy barrier on lyophobic colloidal particles delays

aggregation and the formation of the bulk state, thermodynamically preferred. Picture

taken from [1].

13

1.3 Interaction between colloid particles:

1.3.1 Attractive interactions:

Purely physical attractive interactions between colloidal particles are referred to as

Van der Waals interactions. These interactions are originated by the attraction

between permanent charge distributions (i.e. dipoles, quadrupoles) and the

corresponding induced charge distributions.

As shown in [1] an expression for the potential energy of interaction between two

dipoles as function of the particles separation distance r can be derived:

6

molec

vdW

CV

r (1.5)

Where C is a constant.

From equation (1.5) can be seen that Van der Waals interactions decay very strongly

with the distance and become therefore relevant only at short range.

1.3.2 Repulsive interactions:

At interface separation between colloidal particles and their continuum medium are

very commonly located electrical charges.

In particular, these charges can be brought on colloidal particles surfaces in several

ways: by adsorption of an ionic surfactant or, by acting on the concentration of

potential determining ions.

Regardless how charges are brought on particles surfaces, identically charged

bodies involve electrical repulsive forces between themselves. In order to quantify

these repulsive interactions it is possible to distinguish two regions: in the first, very

close to the particle surface and few nanometers thick, counterions are fixedly

adsorbed on their correspondent ions; in the second at larger distance Brownian

motion dominates and the ions diffuse freely in the electrical field. This picture is

referred to as the Helmoltz double layer (cf. Figure 1-6).

14

Figure 1-6 Helmoltz double layer. Picture taken from [1].

For x>0 the Poisson equation is valid:

2

(1.6)

Where , , are respectively electrostatic potential, medium permittivity and

charge density. can be expressed as

all ions

i i

i

n z e , where in is the number ion

concentration of the ith ion, iz is the valance of the ion and e is the electron charge.

For x>d is valid Boltzmann equation:

0exp( )i

i i

B

z en n

k T

(1.7)

Where Bk is Boltzmann constant and T is the system temperature. Combining

equation (1.6) and equation (1.7) we obtain:

15

2 01

exp( )ii i

B

z ez en

k T

(1.8)

with boundaries conditions: 0 at x (bulk) and d at 0x .

Solving equation (1.8), it is possible to obtain as a function of the distance. What is

generally observed is that at a particular distance defined Debye length, the

electrostatic potential becomes negligible. Physically the ions are completely

screened by the layer of their corresponding counterions. The Debye length is

defined as:

22

B

A

k T

N e I

(1.9)

Where

2 0

2

i iz nI

is the solution ionic strength and AN is the Avogadro number. This

relation highlights a strong potential dependence from the solution electrolyte

concentrations. In particular increasing the electrolyte concentration and so the ionic

strength, decreases meaning that the presence of charge will be perceived a

shorter distances. This phenomenon is known as double layer compression and is

widely used in applications to destabilize colloids.

When two charged bodies approach each other the corresponding double layer

overlap, the local ion concentration increases compared to the bulk, thus creating an

osmotic pressure and therefore a corresponding repulsive force.

Based on this approach several quantitative descriptions have been derived to

evaluate the electrostatic repulsive potential energy RV between two bodies.

1.3.3 DLVO theory

The Derjaguin-Landau-Verwey-Overbeek (DLVO) theory is commonly used to

describe colloidal interactions. DLVO theory is based on the assumption that colloidal

interactions can be explained as combination of attractive forces and repulsive

forces.

16

The total potential interaction energy is so given by the sum of Van der Waals AV and

electrostatic RV potential energy:

tot A RV V V (1.10)

The total potential curve has a number of important features in relation to colloidal

stability (cf. Figure 1-7): it displays an intermediate maximum due to electrostatic

forces that represents a potential energy barrier which has to be overcome for

aggregation to occur; it shows a deep primary attractive well, indicating that Van der

Waals forces dominate at short distances and once aggregation has occurred the

aggregate is difficult to break; it points out that at high distance Van der Waals forces

become relevant again leading to formation of a secondary less deep minimum and

weaker aggregates. To decrease the energy barrier and so to induce aggregation it is

possible acting on the ionic strength causing the compression of the double layer.

Increasing salt concentration leads to a decrease of the potential energy barrier

whose maximum becomes zero (curve d in Figure 1-7). At this point there is no

opposition to aggregation which becomes controlled by Brownian diffusion. The

smallest electrolyte concentration leading to such rapid coagulation is called critical

coagulation concentration (CCC). Mathematically it corresponds to the situation

where 0totV and 0totdV

dD .

17

Figure 1-7 In the middle the total potential as sum of double layer repulsion and van

der Waals attraction (dashed lines). At top right zoom on primary and secondary

minimum. At bottom right effect of salt increase on the potential curve. Picture taken

from [4]

18

1.4 Aggregation

As previously introduced, aggregation is the process in which colloidal particles,

named primary particles, collide between themselves in their continuum medium and

then stick together forming larger aggregates called clusters that can as well again

collide and stick together.

The two main processes bringing particles together are Brownian motion and

convection induced by an external imposed velocity field. The former process is

referred to as stagnant or perikinetic aggregation, the latter as orthokinetic or shear-

induced aggregation (SIA).

Regardless how particles get together, they may or may not stick one to each other

depending on their interaction profile given by the DLVO potential: if no energetic

barrier is present each collision will turn out to be effective. In case of stagnant

conditions where the aggregation process would be dominated only by Brownian

diffusion, this situation is classified as diffusion-limited cluster aggregation (DLCA).

On the other hand, if an energetic barrier is present the particles can repel each other

and every collision will not necessarily lead to an aggregate formation. This situation,

somewhat analogous to the activation process for a bimolecular chemical reaction, is

defined as reaction limited cluster aggregation (RLCA) and can occur in both

stagnant and shear conditions.

During aggregation clusters of different shapes and masses are formed. In order to

describe this distribution, typically broad, mass balances for each cluster must be

written. This mathematical formalism was developed by Smoluchowski under the

hypothesis that clusters breakage is negligible. The corresponding population

balance equations (PBE) read:

1

, ,

1 1

1

2

kk

i k i k i i k i k i

i i

dNN N N N

dt

(1.11)

kN is the number concentration of k-mass aggregates, referred to as cluster mass

distribution (CMD). The first term on the right side of equation (1.11) represents all

the collisions of i,k-sized clusters that lead to the formation of k-sized clusters; the

second term of equation (1.11) is the rate of disappearance of k-sized aggregates

19

with clusters of any mass. ,i k are the aggregation rate constants, expressions for

RLCA, DLCA and SIA will be derived more in details in the following sections.

1.4.1 Diffusion limited cluster aggregation kernel

It is worth to focus on a single fixed (non-diffusing) particle with a hydrodynamics

radius a , which interacts with equally sized, freely diffusing particles. Under the

assumption that upon collision the diffusive particles disappear, the system governing

equation is the continuity equation

( ) 0N

divt

J (1.12)

where F

SJ with F the flux of identical particles diffusing through a sphere with

surface S centered around the reference particle (cf. Figure 1-8).

Figure 1-8 Flux of identical particles diffusing through a sphere centered around a

reference particle.

20

At steady state equation (1.12) becomes

0N

t

(1.13)

And

0div F (1.14)

in case of aggregation entirely controlled by diffusion according to Fick’s law F

expression is given by

28

dNF r D

dr (1.15)

Where D is the self-diffusion coefficient, N the particle concentration and r the

radius of the sphere. Integrating equation (1.15) from bulk condition ( r and

0N N ) to the particle contact point ( 2r a and 0N . ) leads to:

08 (2 )F D a N (1.16)

The total rate of capture per unit volume of the system would be

2

0 0

1 1

2 2

dNFN N

dt (1.17)

Where 0

F

N and the factor 0.5 is used not to count twice the same collision event.

Since the particles are treated as hard spheres, one may express D in terms of the

Einstein-Smoluchowski equation as:

21

6

Bk TD

a (1.18)

Where is the medium dynamic viscosity. becomes

8

3

Bk T

(1.19)

This expression for is valid only in case of identical aggregates sizes and is

referred as ii . In case of different size particles with radii iR and jR can be shown

that (cf. [1]):

2 1 1

4 ( )( ) ( )( )3

Bij i j i j i j

i j

k TR R D D R R

R R

(1.20)

In order to solve PBE in the general case where the aggregation rate is size

dependent ij must be correlated to the masses i and j of the two colliding clusters.

From scattering measurements it has been observed that aggregating clusters exhibit

a self-similar (fractal) morphology and so fd

iR i ,where fd is defined as the fractal

dimension. In particular fd equal to one corresponds to a line, fd equal to two to a

plane and fd equal to three to a sphere (typical values for fd in DLCA are in the

range 1.6-1.9).

It is so finally possible to link ij with i and j obtaining the following expression:

1 1 1 12

( )( )3

f f f fB d d d dij

k Ti j i j

(1.21)

1.4.2 Reaction limited cluster aggregation kernel

In case of perikinetic aggregation where is present a repulsive energy barrier

between particles aggregation is potential-limited. In detail if two diffusing particles

22

interact with one another they experience a force given by their total interaction

potential totV :

tottot

dVF

dr (1.22)

This force is equilibrated by the Stokes friction force fcF Bu where B is the friction

coefficient in a viscous fluid and u the particle speed.

It is possible to show that the expression for the flux F becomes so:

28 ( )tot

B

dVdN NF r D

dr k T dr (1.23)

Integrating equation (1.23) at steady state from bulk condition ( r , 0N N . and

0totV ) to the particle contact point ( 2r a and 0N ) leads to:

0

22

8tot

B

V

k T

a

DNF

dre

r

(1.24)

It is worth to point out that if 0totV in the whole domain we obtain the same

previous DLCA flux. (defined asF

N) can be extended to RLCA. It becomes so

possible compare DLCA kernel with RLCA:

2

2

2tot

B

VDLCA RLCAk T

a

F drW a e

F r

(1.25)

The parameter W defined as Fuchs stability ratio gives crucial information about how

distant in term of stability is the system from its most unstable configuration: if W =1

the system is fully destabilized; if W increases the stability improves.

The meaning of W can be more appreciated in relation to the system salt

concentration and its most important effect: the double layer compression.

23

Looking at the region in Figure 1-9 where W >1 can be observed that increasing the

salt concentration leads to a less stable situation until in the region where W =1 the

system is completely under diffusion control. It is important to note that the

intersection of the two straight lines indicates the CCC value, where the energy

barrier vanishes.

Figure 1-9 Typical profile of the Fuchs stabil ity ratio as function of the salt

concentration. Picture taken from [5]

The earlier comparison between DLCA and RLCA kernel was obtained only

considering primary particles. To extend this to the aggregation of two clusters with

sizes i and j the interaction aggregate-aggregate can be approximated with the

interaction between the two colliding primary particle (described by the stability ratio

W ) and the rate of aggregation can be assumed proportional to the probability of

collision between primary particles on the cluster surface.

For a given k-mass cluster the change in the primary particles in the cluster with is

size ka is given by:

1

1( ) ( )

f

f f f

d

d d df fk k

k

d da adkk k

a da a a a

(1.26)

The final expression for RLCA kernel results so:

( )

DLCA

ijRLCA

ij ijW

(1.27)

24

Where 1f

f

d

d

(typical RLCA fd are in the range 2-2.2). More in general is

obtained by fitting experimental data.

1.4.3 Shear induced aggregation kernel

The most general situation in orthokinetic aggregation is when the diffusing particles

are immersed in an external speed field and their DLVO potentials totV interact with

one another [6].

The expression for F is given by (cf. [6]):

tot

B

NDF V Bu D N dS

k T

∮ n (1.28)

Equation (1.28) if inserted in the continuity equation (equation (1.12)) leads to a

three-dimensional space partial differential equation that cannot be solved

analytically. However since our problem is to determine the collision frequency the

equation can be reduced to an ordinary differential equation in the radial distance as

the independent variable. Integrating under the proper boundary conditions (cf. [6])

equation (1.28) becomes:

0

20

16

12 [ ]

( )( 2)

xtota

eff

a B

DaNF

dVdxexp dx Pev

x x k T dx

(1.29)

Where is the thickness of the hydrodynamic boundary layer, x is the surface to

surface radial distance between particles, ( )x is an hydrodynamic functions

accounting for the resistance of the solvent being squeezed when two particles

approach each other, effv is the relative velocity between two particles normalized by

a ( is the shear rate [1/s]) and Pe is the Peclet number (the ratio between shear

and Brownian forces)

25

33

B

aPe

k T

(1.30)

A more generalized expression for the stability ratio W valid for arbitrary Pe

numbers and interaction potentials can be obtained:

2

0

12 [ ]

( )( 2)

xa

toteff

B

a

dVdxW exp dx Pev

x x k T dx

(1.31)

The integrals in equation (1.31) need again to be evaluated numerically. Further

approximations can be done by considering high interaction potential barrier and

moderate Peclet numbers. These simplifications lead to a loss of accuracy in the

calculation and allow only a proportional relation (cf. [6]):

2

B

mVPe

k TW e

(1.32)

Where mV is the value of the potential and evaluated at the maximum of the

interaction potential; is a geometric parameter. From the W expression can be

evaluated the shear induced aggregation kernel which is given by

2

B

mVPe

k TSIA

ij e

(1.33)

Finally a characteristic time for binary encounters can be introduced. This is referred

to as characteristic time of aggregation and is defined as:

0

agg DLCA

W

N

(1.34)

26

1.5 Gelation

In viscous liquid dispersions with solid volumetric fraction higher than 1% aggregation

processes end most of the times in the formation of a viscoelastic solid phase,

usually referred as colloidal gel. After clusters are formed, due to the ongoing

aggregation, they continuously grow in time as long as they interconnect with one

another and thus create a network which occupies all the dispersion available volume

(cf. Figure 1-10).

Figure 1-10 Steps of gel formation. Picture taken from [1].

In order to identify the condition at which the system gel can be introduced the

volume fraction of cluster at time t :

34( )

3i i

i

t N R (1.35)

Where iN is the cluster mass distribution and iR , is the smallest sphere radius

containing the aggregate. When t reaches 0.5 half of the dispersion volume is

occupied by cluster that cannot freely move any more. At this point where

interconnection starts the system stop behaving like a viscous liquid becoming a

viscoelastic solid able to sustain applied external stresses. The gel time gelt depends

on the regime at which gelation takes place: in DLCA there is no energy repulsion

and the CMD is rather mono-disperse (all clusters experience the same environment

and are on average separated by the same short distances) so the gelation process

is very fast; in RLCA the interconnection process is not instantaneous because of the

energy barrier and the super poly-disperse CMD which decreases the diffusion speed

since clusters of different sizes obstruct one another.

27

1.6 Coalescence

Coalescence is the process in which the dispersed phase is a fluid. The liquid

droplets join together fusing in larger droplets and in so doing destroy interfacial area.

In order for particles to coalesce, they first need to approach closely enough to

aggregate, then they interdiffuse in one another, melting in a single droplet (cf. Figure

1-11).

Figure 1-11 Steps of coalescence: approach, aggregation and finally coalescence.

A characteristic time of coalescence was introduced by Frenkel [7]:

p

coal

d

(1.36)

Where p is the particles viscosity, d the diameter of the final sphere and the

surface tension.

Coalescence strongly affects the final shape of clusters. In fact if its characteristic

time is comparable with the time of aggregation spherical cluster are formed and in

this case no gelation can occur.

In polymeric dispersions coalescence can occur only if the system temperature is

above the material glass transition temperature gT . In fact above gT a non-crystalline

polymer material behaves rubbery or like a viscous fluid, depending on how much the

temperature exceeds the gT ; below gT a bulk polymer shows hard-solid material

features.

28

2 SAMPLES PREPARATION:

2.1 Synthesis:

2.1.1 Materials:

Four samples of poly(methylmethacrylate-co-butylacrylate) P(MMA-co-BA) have

been synthesized by starved emulsion polymerization in a semi-batch reactor. These

samples are copolymers produced at different mass ratios (Table 2-1) of methyl

methacrylate (MMA) and butyl acrylate (BA) (cf. Figure 2-1)

Figure 2-1 Left methylmethacrylate molecule; Right butylacrylate molecule

Table 2-1 Mass ratios of MMA and BA for each sample

PMMA-co-BA

%MMA

%BA

SAMPLE 1 30 70

SAMPLE 2 50 50

SAMPLE 3 60 40

SAMPLE 4 70 30

Henceforth every sample will be identified by referring only to its MMA content.

MMA and BA were supplied by ABCR CHEMICALS with purities of 99% and were

used as received.

29

During the polymerization Sodiumdodecylsulfate (SDS) and Potassiumpersulfate

(KPS) were used as surfactant and initiator respectively (cf. Figure 2-2).

Figure 2-2 Top Sodiumdodecylsulfate; bottom Potassiumpersulfate

The amounts of SDS and KPS relative to each sample are listed in Table 2-2:

Table 2-2 Amounts of SDS and KPS relative to each sample

%MMA

SDS [g]

KPS [g]

30 0.291 0.815

50 0.275 0.815+0.4

60 0.227 0.815

70 0.207 0.815

SDS with purity >99% was provided by Apollo scientific; KPS with purity >99% was

provided by Sigma-Aldrich. Both were used as received.

It is worth to point out that in each synthesis the nucleation was homogenous; in fact

surfactant amount did not exceed the CMC (from the literature 6-8 [mM] at 25 [ºC]).

Deionized water previously stripped for 40 minutes with nitrogen (in order to remove

oxygen) was employed as continuous phase in the polymerization.

30

2.1.2 Equipment:

The polymerization was run round bottom flask of 1000 ml. Four openings were

present on the top of this flask: one was used to connect it with a water condenser,

all the others were sealed with septums.

These caps were able to avoid air entry and to allow the feed through capillaries of

the monomer using a volumetric pump and of the nitrogen.

Temperature and mixing control were achieved through a programmable heating

plate, in particular a thermocouple linked to the heating plate.

2.1.3 Protocol:

SDS was initially charged into the reactor dissolved into 673 [ml] of water

(approximately with a ratio SDS/ water of 0.04%)

The mixture was heated to 70 ºC and stirred at 800 r.p.m.

KPS dissolved in 40 [ml] of water, once the temperature was reached and

stabilized for 20 minutes, was added (approximately with a ratio KPS/ water of

0.19-0.12%)

After temperature stabilization 10 minutes the monomers feed (0.285 [ml/min])

was started

Samples were taken during the polymerization in order to monitor conversion,

particle size, particle polydispersity (PDI), and dry content (DC); as soon as

DC>5% and the sample particles reached sizes of circa 200 [nm] the feed was

stopped

The latex was kept at 70 ºC for one hour in order to guarantee a complete

monomer conversion

During the whole polymerization the reactor was purged with nitrogen

Exception: the polymerizations of the 50% MMA lasted longer than five hours so it

was necessary to add after five hours 0.4 [g] of KPS dissolved in 20 [ml] of water in

order to guarantee a continuous radicals production.

During sampling after circa one hour only unitary conversion were measured. At the

end of the polymerization every sample was cooled and filtered with filters paper.

The final sizes, PDI and dry contents of the samples are reported in Table 2-3.

31

Table 2-3 Samples final particles average diameter, polydispersity index and dry

content

%MMA

Average diameter [nm]

PDI [-]

DC [%]

30 198 0.027 9.73

50 188 0.016 13.44

60 199 0.017 9.42

70 198 0.021 9.48

Sizes and PDI measurements were performed by dynamic light scattering DLS.

It is relevant to note that the PDI index (dimensionless measure of the broadness of

the size distribution) is not defined as common. In the DLS software it is calculated by

cumulant analysis and it ranges from 0 to 1. Zero value stands for completely mono-

dispersed samples whereas one for very poly-dispersed ones. Values of PDI<0.05

are normally encountered with monodisperse latexes.

2.2 Purification:

2.2.1 Materials:

In order to purify the latexes from the ions (surfactant, sodium and potassium) an ion

exchange resin was used. Ion exchange is the reversible interchange of ions

between a solid (ion exchange material) and a liquid in which there is no permanent

change in the structure of the solid. Conventionally ions exchange resins consists of

a cross-linked polymer matrix with a relatively uniform distribution of ion-active sites

throughout the structure [8].

The ion exchange resin used as received in our application was Dowex Marathon

MR-3 hydrogen and hydroxide form 20-50 mesh, provided by SIGMA ALDRICH.

On this resin matrix are present both cationic H+ and anionic OH- sites so all the

target ions were removed.

32

In order to check the effective removal of surfactant the interfacial tension of each

purified latex was measured with a dynamic contact angle meter and tensiometer

(supplied by DATAPHYSICS).

2.2.2 Protocol:

An amount of resin between 10-20% of the latex mass was added to the

sample to purify

The resin was removed by filtrating the solution with 50 [μm] and 5 [μm] filters

5 [ml] of the sample where diluted in 50 [ml] of water and the interfacial tension

was measured

The protocol was repeated until the values of γ were comparable with the one of pure

water (73 [mN/m]). The final γ values are listed in Table 2-4.

Table 2-4 Samples f inal γ values

%MMA

γ [mN/m]

30 71.89

50 72.02

60 72.34

70 72.21

At the end of the purification in order to check if aggregation occurred the sizes of all

the samples were measured. No appreciable differences were found.

33

2.3 Composition control:

2.3.1 Equipment: Differential scanning calorimetry

Although starved emulsion polymerization assured an excellent composition control,

further composition verifications can be carried out by measuring the samples glass

transition temperatures. From the literature it results a gT of 105 ºC for the pure MMA

polymers and of -43 ºC for the pure BA ones; changing in the intermediate samples

the composition ratio MMA/BA should lead to a gT gradient among these two

temperatures (cf. Table 2-5).

Differential scanning calorimetry (DSC) is one of the most effective methods of

determining glass transition temperature. The basis of DSC is the change in the

specific heat of a polymer due to the change of temperature as it passes through the

glass transition point; particularly the heat capacity increases at gT going from

amorphous solid to viscous liquid.

In a typical DSC experiment [9], two pans (one contains the polymer and the other is

empty [reference pan]) are placed in an inert atmosphere on a pair of identically

positioned platforms connected with a heating system. The two pans are heated up

at exactly the same specific rate despite the fact that one pan contains polymer and

the other one is empty. In order to keep the temperature of the sample pan

increasing at the same rate as the reference pan more heat is required; so it is

possible to plot this difference in the heat flow as a function of temperature.

When there is no glass transition in the polymer, the heat flow in the plot is parallel to

the x-axis; when the glass transition temperature is reached the heat flow shows an

increased slope. Usually as gT is taken approximately the middle of the increased

slope. For the analysis was used the DSC Q200 provided by TA INSTRUMENTS.

The pan material was aluminum.

2.3.2 Protocol:

10 ml of each sample have been dried one night at 45 [ºC] in an oven with the

vacuum open

34

5-10 [μg] of sample have been inserted in the DSC machine for the analysis

As heating rate was used 10 [ºC/min] and the interval scanned was of 100

degrees centered on the theoretical expected gT

gT curves are reported in APPENDIX I, the final results are listed in Table 2-5

Table 2-5 gT values for each sample

%MMA

gT [ºC]

30 -12.3

50 17.3

60 35.7

70 54.4

35

3 SAMPLES CHARACTERIZATION:

3.1 Light scattering

Amongst many experimental techniques available to investigate colloidal systems

and aggregation phenomena light scattering measurements are the most efficient in

terms of accuracy and non-intrusiveness [10].

When particles are irradiated by electromagnetic waves of wavelength comparable or

larger than the size of the particles themselves an oscillating dipole is formed. As the

dipole changes they scatter the radiation in all directions (cf. Figure 3-1).

Figure 3-1 Incident l ight scattered by a particle

3.1.1 Static light scattering theory:

Static light scattering (SLS) is a light scattering technique that operates measuring

the scattering intensity I , intended as the sum of all the radiations scattered by the

element, at every angle and at a fixed distance from the scattering center.

From the spectrum analysis of the scattering intensity is then possible to gain crucial

information regarding the dispersion and the aggregates structure, in fact I is

sensitive in general to the particles size, structure…

At the basic of the conventional SLS theory for colloidal dispersion (Rayleigh-Debye-

Gans) [11] there are the assumptions that electromagnetic radiations are identically

scattered only once (the contribution of multiple scattering is neglected), only the

36

incident radiation is considered and the difference of refractive index between the

particles and the medium is not too large.

Experimentally these conditions can be achieved working at very low concentrations.

Generally the intensity is expressed as function of the scattering wave vector in place

of :

04sin

nq

(3.1)

Where 0n is the refractive index of the dispersion medium and is the radiation

wave length in the vacuum. The importance of this vector is that its inverse 1q

represents the length scale of the scattering experiment.

The scattered intensity can be expressed as the product of different factors [1]:

2

0 1 pI q I K NV P q S q const P q S q (3.2)

0I is the intensity of the incident radiation. 1K is a constant which incorporates the

dependence on the optical constants. N is the number of identical cluster per unit

volume; pV is the particle volume. P q , defined as form factor, describes the

scattered intensity from a single primary particle and depends only on its shape and

size; in case of spherical particles smaller at last ten times smaller than the

wavelength of radiation the form factor is given by [1]:

2

3

3 (sin cos( ) )

( )

p p p

p

qR qR qRP q

qR

(3.3)

It is worth to point out that 0

lim 1q

P q

. S q , defined as structure factor, depends on

the correlation among the particles in the aggregate: for primary particles it results

everywhere 1S q ; for self-similar aggregates is valid in the fractal region

~ fdS q q

.

37

In general 2

0 1 pI K NV is a constant: in case of primary particles, since at 0q we have

1P q and 1S q , it can be directly determined from the intensity profile

2

0 10 (0) pI q I I K NV ; in case of cluster and poly-disperse cluster the quantity

(0)I must be in general extrapolated. Dividing (0)I of primary particles by 0I

allows determining P q .

In case of aggregation the structure factor S q changes in times due to the growth

in size and the change in structure of the aggregates. Dividing the scattering intensity

spectrum by P q allows to obtain the structure factor of the aggregate S q and so

indirectly from the power the fractal dimension.

Another very important quantity that can be obtained by the scattering profile is the

radius of gyration gR , defined as the sum of the squares of the distances of all the

cluster particle from its mass center. It can be determined by a linear fitting of 0I

using the so called Guinier plot analysis (cf. [11]):

2 2 2 21 1

log log( ) log 10 3 3

g g

I qP q S q q R q R

I

(3.4)

Where the approximation log 1 x x has been used in equation (3.4).

Our analysis have been performed in MALVERN MASTERSIZER 2000, particularly

several kinetics of aggregation in stagnant DLCA have been carried out.

3.1.2 Protocol:

Measurements of P q :

Each sample was diluted in pure deionized water at 5x10-5 in volume fraction

A proper amount of a 2 [M] NaCl solution was added to reach the final

concentration of 10 [mM] NaCl

38

All the intensity data have been treated as previously explained in order to get the

final expression of P q . 10 [mM] NaCl are experimentally suggested in order to

reduce the Debye length of the cleaned samples and so to allow diffusion avoiding

structure effects (In case of no salt the particles feel a too long range their mutual

interaction and have less space in which can diffuse).

Aggregation kinetics:

Each sample was diluted in pure deionized water (where previously air

bubbles were removed) according to the final volume fraction and salt

concentration

The necessary amount of a 5 [M] NaCl solution (where previously air bubbles

were removed) was poured into the latex solution

This protocol was adopted in order to avoid mixing the latex with a highly

concentrated salt solution which could have induced locally fast aggregation, spoiling

so the consequent kinetic measurements.

High final NaCl concentrations were used in order to have density matching between

the solutions and growing aggregates preventing so sedimentation.

3.1.3 Dynamic light scattering theory:

In dynamic light scattering (DLS) measurements the scattered light intensity I is

monitored at one fixed angle θ and at a fixed distance from the scattering center.

More in detail, since the particles in the dispersion undergo to Brownian motion and

so their mutual position change on a time scale, the observed scattering intensity

exhibits fluctuations. From the rate of decay of these fluctuations information about

the diffusion rate and so about the particles sizes (once the diffusion coefficient is

known the hydrodynamic radius can be easily evaluated for spherical particles

6

Bh

k TR

D ) can be extracted; it is evident in fact that the more the particles diffuse

and so the smaller they are, the higher will be the fluctuation frequency. Such

39

fluctuation can be analyzed defining a correlation function which takes into account

the intensity self-correlation between time 0 and . This function is defined as follow:

2

2

,0 ,1 D q

I q I qg Ae

I q

(3.5)

Where A is a constant depending on the experimental set-up.

Once the correlation function is experimentally built D can be obtained by fitting with

cumulant analysis the right member term expression with the left one.

Two different DLS machines were used: BROOKHAVEN and MALVERN

ZETASIZER. The angles at which measurements were taken are respectively 90º

and 173º. The same experimental protocol of SLS was used for DLS measurements.

3.2 Titration

3.2.1 Theory:

On the surfaces of our latex particles fixed negative charges (sulfate groups) are

present as KPS was used during the polymerization.

By far the most commonly used method to count the number of fixed groups is

provided by conductometric titration.

In fact for each acid site there is a corresponding H+ associated. Measuring the

amount of H+ in the system gives the amount of sulfate groups and therefore the

fixed charges amount.

In a conductometric titration a titrant (in our case NaOH) is added to the colloidal

dispersion and the conductivity is monitored.

At first as the titrant is added, the conductivity decreases because the more

conductive (mobile) ions H+ are replaced by the less mobile Na+ ions and then are

neutralized with the OH- ions.

Once all the ions H+ associated with the surface groups are neutralized, further

addition of base just increase the total electrolyte content of the solution leading to a

raise in conductivity.

40

The breakpoint extrapolated from the two slopes gives the number of sulfate sites

(the amount of titrant added is in fact known).

3.2.2 Protocol:

5 [g] of sample were diluted in 50 [g] of deionized water previously stripped

with nitrogen ( in order to avoid the effect of the eventually dissolved CO2)

0.5 [ml] of 0.1 [M] solution of NaCl were added in order to promote the

replacement mechanism. At each step 0.05 [ml] of a 10 [mM] NaOH were

added to the solution and then the conductivity was measured

During all the titration time the samples were gently stirred and continuously stripped

with nitrogen.

The results of the titrations are reported in Table 3-1

Table 3-1 Surface charges for each sample

%MMA

σSO4 [mol H+/KgPolymer]

30 0.01607

50 0.00896

60 0.01064

70 0.00931

3.3 ζ-potential

3.3.1 Theory:

If an external electric field is applied to charged particles in dispersion, phenomena

associated with the relative movement of charges (i.e. electrokinetic) are possible.

These phenomena are referred to as electro-osmosis, if the liquid moves and the

solid is stationary, and electrophoresis, the opposite phenomenon [10].

41

If the particle size is larger than the double-layer thickness and a coordinate system

referred to the solid particle is chosen electro-osmosis and electrophoresis can be

described essentially as the same phenomenon. Only one description is so required

and electro-osmosis will serve the purpose [10].

In details a double-layer thickness much smaller than the particle size allows to

approximate the particle surface as a flat one (cf. Figure 3-2); considering then a

coordinate system referred to the solid particle allow to consider the liquid in motion

around it.

The final objective of this representation is to derive an expression for the velocity

profile v on the particle surface and in particular its value in bulk eV .

Figure 3-2 Velocity profile on a negatively charged particle surface. In the inner part of

the double layer were counter ions are fixedly adsorbed on their correspondent ions

(slip plane) the velocity profile is zero and the potential is equal to the value of the -

potential.

It can be demonstrated [10] that this is given by:

e

EV

(3.6)

Where is the dielectric constant, the medium viscosity, E the intensity of the

electric field and is the so called -potential. The -potential is the value of the

potential very close to the particle surface (slip plane) where the velocity profile is

equal to zero.

42

Changing coordinate system from the solid particles to the continuum medium leads

to find particles moving by effect of the electric field at speed p eV V .

This velocity or more exactly the electrophoretic mobility pVu

E (so also the -

potential) can be directly measured by combining DLS and electrophoresis

techniques.

In our case was used a MALVERN ZETASIZER.

3.3.2 Protocol:

The necessary amount of each sample was diluted at 1x10-5 volume fraction

and at the target salt concentration of NaCl mixing at first the salt with water

and then adding the latex.

In case of measurements at 45 [ºC] the samples were pre-heated in an oven

and equilibrated for 5 minutes in the Zetasizer

Results are listed in Table 3-2 and Table 3-3

Table 3-2 ζ -potential values at 10 [mM] NaCl

%MMA

ζ -potential [mV]

25[ºC] 45 [ºC]

30 -73.23 -62.66

50 -57.8 -55.6

60 -59.8 -61.66

70 -45.8 -55.16

43

Table 3-3 ζ -potential values at 140 [mM] NaCl

%MMA

ζ -potential [mV]

25[ºC] 45 [ºC]

30 -42.26 -40.13

50 -33.9 -30.5

60 -31.33 -28.76

70 -27.63 -26.4

3.4 Rheometer

3.4.1 Theory:

A rheometer is a device capable of applying controlled shear to a colloidal dispersion.

Our instrument consisted in an outer rotating cup and an inner fixed cylinder (cf.

Figure 3-3). This particular configuration, referred to as Couette geometry, was

employed because it guarantees to obtain between the moving and fixed solid

surfaces a steady laminar and isothermal flow of the dispersion [12].

Figure 3-3 Schematic of a rheometer Couette geometry. The sheared dispersion (blue)

l ies between the cup (outer rotating part) and the bob (f ixed inner cylinder).

Bob (inner fixed cylinder)

Cup (outer rotating part)

44

In detail a rheometer measures the angular deflection of the fixed part which

indicates the torque on the bob.

By measuring this stress the viscosity of the system can be easily monitored on time,

for Newtonian fluid is valid in fact [12]:

shear (3.7)

Where shear is the shear stress. For non-Newtonian fluids relations similar to

equation (3.7) are available in the literature.

An ARES rheometer was used for the analysis. The temperature was controlled with

a thermal bath. The outer fixed part diameter was 33.3 [mm], the inner cup diameter

was 34 [mm]. A gap of 3 [mm] from the bottom of the rotating cup was used in order

to avoid border effects. Since aggregation alone under shear can occur on very large

time scales small amount of salts were added to fasten the process.

3.4.2 Protocol:

The sample were diluted at first with the proper amount water and then with a

2 [M] NaCl solution in order to reach a final dry content and the target salt

concentration

After mixing the latex with the salt solution the size was checked in DLS and if

no variations were observed the analysis were started

The rheometer turned up to be a very sensitive system. In order to achieve

reproducible experiments a very strict cleaning procedure must be followed:

Wash the cup and bob with deionized water and soap

Wash the cup and bob with methyl-ethyl-ketone

Clean the cup and bob with deionized water and soap

Keep the cup and bob in 0.5 [M] H2SO4 solution for at least 10 minutes

Wash the cup and bob with deionized water and soap

Dry the cup and bob with nitrogen

45

4 RESULTS AND DISCUSSION

The present work purpose is to understand the role that coalescence plays in the

aggregation under shear.

In general sheared dispersions are a very complex system to analyze; their

aggregating behavior involves several physical phenomena: the particles are

diffusing immersed in an external speed field and are interacting with one another

according to the attractive and repulsive forces they are subjected to (i.e. their

interaction potential).

Therefore, it was initially necessary to understand their interaction potential in

stagnant conditions and only later shear conditions were explored.

In particular, aggregations induced by salt (NaCl) were performed in stagnant DLCA

conditions at different latexes volume fractions ( =1-3x10-5 and 0.05-0.1)and

temperatures (25-45 [ºC]).This temperature range was examined as it enabled

coalescence (which occurs only above the material glass transition temperature) for

some of the samples (cf. Table 2-5). Low volume fractions were tested since smaller

particles concentration increase the characteristic time of aggregation (cf.

equation(1.34)) and allow to clearly observe the effects of coalescence ( coal <<agg ).

Higher volume fractions were analyzed, although the characteristic time of

aggregation ( coal >>agg ) is very small in those cases, in order to elucidate the

mechanism of gelation of different samples in stagnant conditions. Note that

comparable particle volume fractions were then employed in shear conditions.

The RLCA experiments were performed in order to better understand the role and

nature of the particle interaction potential on particle aggregation. Surface charge, ζ-

potential and light scattering measurements were performed in order to deepen this

point.

Finally shear aggregations were performed in the rheometer with a fixed dry content

(DC=5%) and shear rate (4900 [1/s]); in these conditions the salt concentration and

temperature were changed in order to clarify the interplay of coalescence and

aggregation.

46

4.1 Stagnant Aggregation

4.1.1 DLCA:

4.1.1.1 Characterization at low volume fractions:

The interplay between coalescence and aggregation was at first investigated in

DLCA by carrying out several salt-induced aggregation kinetics in the small angle

static light scattering at =1x10-5, 2x10-5, 3x10-5. The SLS temperature and final

NaCl concentration were in all cases respectively 30 [ºC] and 4 [M] (This high salt

concentration was employed in order to have density matching between the solution

and the aggregates, avoiding their sedimentation). The results of the aggregation

kinetics (in terms of gyration radius gR versus time) are reported in Figure 4-1,

Figure 4-2 and Figure 4-3.

Working at low primary particles concentration increases the characteristic time of

aggregation.

Figure 4-1 Gyration radii evolutions of 70-30% MMA samples as function of t ime at

1x10-5

0 50 100

0.0

0.5

1.0

1.5

2.0

2.5

3.0 70% MMA

60% MMA

50% MMA

30% MMA

Rg [

m]

Time [min]

Rg

47

Figure 4-2 Gyration radii evolutions of 70-30% MMA samples as function of t ime at

2x10-5

Figure 4-3 Gyration radii evolutions of 70-30% MMA samples as function of t ime at

3x10-5

0 50 100

0.0

0.5

1.0

1.5

2.0

2.5

3.0

3.5

4.0 70% MMA

60% MMA

50% MMA

30% MMA

Rg [

m]

Time [min]

Rg

0 50 100

0.0

0.5

1.0

1.5

2.0

2.5

3.0

3.5

4.0

4.5

5.0 70% MMA

60% MMA

50% MMA

30% MMA

Rg [

m]

Time [min]

Rg

48

In particular in DLCA agg can be evaluated since in equation (1.34) W is equal to

one:

0 0

1agg DLCA DLCAN

W

N

(4.1)

Table 4-1 agg values evaluated at 1x10-5

, 2x10-5

, 3x10-5

agg [s]

1x10-5 45

2x10-5 22

3x10-5 15

Increasing the characteristic aggregation times allows the particles in the aggregates

(if they can) to coalesce ( coal agg ). The main effect of coalescence during these

aggregation kinetics would be the formation of spherical-similar aggregates ( fd =2.4

– 3) with smaller gyration radii compared with the non- coalescing ones.

Focusing on the gyration radii it can be seen from Figure 4-1, Figure 4-2 and Figure

4-3 that the 70% MMA and 60% MMA ones completely overlap.

Notably, the 70% MMA and 60% MMA particles at these experimental conditions are

below their gT (cf. Table 2-5) and so exhibit hard-solid material features, in

particularly their viscosity diverges to infinite. As a consequence their corresponding

characteristic times of coalescence, defined in equation (1.36), diverge to infinite and

coalescence cannot occur. These gyration radii are therefore evolving at the

maximum rate according to the DLCA aggregation regime.

Figure 4-1, Figure 4-2 and Figure 4-3 show that the 50% MMA and 30% MMA radii of

gyration are progressively smaller than the 70% MMA and 60% MMA ones. Notably

the 50% MMA and 30% MMA particles at these experimental conditions are above

their gT (cf. Table 2-5) and so behave like viscous fluid with a well-defined and

progressively lower viscosity. Therefore coalescence occurs for these samples: as

expected the higher the BA content, the faster coalescence occurs.

49

Additional evidences for the 50% MMA and 30% MMA particles coalescence can be

gained looking at a more universal behavior of the aggregating system: introducing

the dimensionless time defined as

0

8

3

Bad

agg

t tNt

W

k T

(4.2)

it results from the literature [13] [14] that when the aggregates radii are plotted

against the dimensionless time defined in equation (4.2) independently of

temperature, primary particles concentration 0N and stability W , they collapse to

form a unique curve known as master curve [14]. In particular, this universal behavior

can be appreciated for DLCA aggregating system looking at the PBE dimensionless

equations:

1

, ,

1 1

1

2

i

i j ji

j i ji j i j

ad j j

X XdX

B X Bdt

X

(4.3)

where

0

iiX

N

N (4.4)

1 1 1 1

1( )( )

4

f f f fd d d d

ij i jB i j

(4.5)

As in DLCA conditions the fractal dimension is fixed once the particle size is defined

[15], it results that the dimensionless CMD (and therefore all resulting averages) are

the same for all the aggregation processes, disregardful of particle concentration and

temperature.

As comparable sizes lead to similar fractal dimensions and the number of primary

particles per cluster is the same, overlapped gyration radii should be obtained

according to the fractal scaling expression (cf. with equation (1.26)):

50

( ) fdg

f

Ri k

a

(4.6)

where 2.084.46f fk d depends only on the fractal dimension and not on the material

[16].

Figure 4-4 reports all the gyration radii kinetics at 1x10-5, 2x10-5, 3x10-5 plotted

against the dimensionless time. As it is shown, for each sample the gyration radii are

overlapped regardless of the volume fraction. As expected the 70%MMA and

60%MMA gyration radii are superimposed while the 50%MMA and 30%MMA ones

remain lower: once more this indicates how coalescence becomes more relevant

while increasing the BA content.

Figure 4-4 Aggregation kinetics of 70-30% MMA samples as function of dimensionless

time at different volume fractions 1x10-5

, 2x10-5

, 3x10-5

Further insights about coalescence can be gained looking at the structure of the

aggregates from SLS fractal dimension measurements.

As previously discussed fd values can be obtained by the SLS intensity curve in the

fractal region with the relation ~ fdS q q

.

51

At the beginning of each aggregation, due to the very low concentrations, self-similar

structures were not yet formed so fractal dimensions increasing in time were found.

When finally fractal aggregates were formed, fractal fd constant in time were found.

These values are reported in Table 4-2. Moreover due to the very low volume

fractions in case of the 30% MMA kinetics the S q analysis could not be performed

since the coalesced particles were too small and consequently the fractal region was

not large enough to extract safely fd values. As shown in [17] another method to

obtain fd is available: it consists in plotting on a logarithmic graph 0I and gR

respectively as y-axis and x-axis and extracting fd as the value of the exponent in a

power regression between these data ( 0I vs. gR plots are reported in APPENDIX

II). fd values extracted with both methods are listed in Table 4-2.

Table 4-2 Values of fd from ( )S q and (0)gR I analysis:

fd

Φ 1x10-5 2x10-5 3x10-5

SAMPLE ( )S q (0)gR I ( )S q (0)gR I ( )S q (0)gR I

30%MMA - 2.45 - 2.33 - 2.98

50%MMA 1.77 1.77 1.8 1.78 1.8 1.86

60%MMA 1.73 1.86 1.74 1.73 1.78 1.87

70%MMA 1.81 1.77 1.8 1.87 1.8 1.72

fd values obtained with the S q analysis are generally comparable with the 0I

vs. gR ones. In case of the 30% MMA were found fd 2.3, additional evidences that

coalescence occurs for this sample.

The only critical issue are the 50%MMA fd : these fd are comparable with the

60%MMA and 70%MMA. If coalesce occurs for this sample, as previously discussed,

52

higher fd would be expected. This inconsistency can be explained with a lag time

between coalescence and the fd measured. At the beginning of the sintering the

50%MMA aggregates present a very open branched structure according to the DLCA

regime; coalescence occurs on the ramified aggregates branches shrinking them and

so decreasing the relative gyration radii. This internal restructuring which strongly

affect the gyration radii slowly changes the overall structure which results therefore in

time only slowly increasing in fd (cf. Figure 4-5).

Figure 4-5 Depiction of the internal coalescing aggregates restructuring: the radius of

gyration changes faster than the overall aggregate shape. Picture taken from [18]

For the 30%MMA this lag time between coalescence and the fd measured has not

been observed. The reason is that the sample characteristic time of coalescence is

much smaller than the 50% one and so a faster coalescence occurred.

Faster coalescence occurs the higher the sample temperature overshoots its gT until

eventually a maximum final rate is reached. The reason is due to the viscosity which

plays a crucial role in the characteristic time of coalescence (cf. equation (1.36)): as

the temperature increases the particles viscosity decreases reducing the

characteristic time of coalescence.

In order to prove the previous statement, several salt-induced aggregation kinetics

were performed in the DLS at 1x10-5 and 4 [M] NaCl. Our available DLS device

allowed investigating the temperature range [25-45ºC]. In these conditions only the

30%MMA, 50%MMA and 60%MMA samples were tested since, according to their

53

relative gT plot listed in APPENDIX I, are the only ones at which the glass transition

occurs. The respective results (in terms of hydrodynamic radius hR versus time) are

reported in Figure 4-6, Figure 4-7, Figure 4-8.

As consequence of faster coalescence, Figure 4-7 shows that increasing the

50%MMA sample temperature over its gT value (17 [°C]) leads to a progressively

smaller hydrodynamic radii evolution.

Figure 4-6 30% MMA hydrodynamic radii evolutions as function of dimensionless time

at different temperatures [25-35º] and at volume fraction 1x10-5

54

Figure 4-7 50% MMA hydrodynamic radii evolutions as function of dimensionless time

at different temperatures [25-45º] and at volume fraction 1x10-5

Figure 4-8 60% MMA hydrodynamic radii evolutions as function of dimensionless time

at different temperatures [25-45º] and at volume fraction 1x10-5

55

A similar trend it is observed for the 60%MMA sample in Figure 4-8. In this case it is

worth to point out that below the 60%MMA gT (35 [°C]) the corresponding

hydrodynamic radii are not overlapped. The reason is that the glass transition does

occur in a region of temperature centered around the glass transition temperature

and not at single fixed temperature as for example for a phase transition. In this

region therefore the particles viscosity can be well defined even below the gT value.

Figure 4-6 exhibits the maximum rate of coalescence which is reached once the

hydrodynamic radii coalesce at their maximum speed rate. This maximum rate of

coalescence it is reached only by the 30%MMA since at the experimental condition

investigated is already fully coalesced ( gT =-12 [°C]).

Further information about the samples relative rate of coalescence can be obtained

comparing the 30%MMA, 50%MMA and 60%MMA aggregation kinetics (cf. Figure

4-9). The 50%MMA hydrodynamic radii at 45 [°C] are superimposed with the

30%MMA ones. This means that the 50%MMA sample in this condition is coalescing

at the same rate of the 30%MMA. Therefore these two samples become comparable

from the coalescence point of view only over 45 [°C].

Figure 4-9 30%-60%MMA hydrodynamic radii evolutions as function of dimensionless

time at different temperatures [25-35º] and at volume fraction 1x10-5

56

Finally, since it has been figured out that the 30%MMA and 50%MMA samples at 30

[°C] are coalescing, hypothesis concerning the respective characteristic times of

coalescence can be formulated (only hypothesis can be put forward due to the nature

of equation (1.36) which results only as proportional relation and therefore does not

allow exact evaluations). These characteristic times can be inferred looking at the

characteristic time of aggregation listed in Table 4-3. As the 30%MMA sample is

clearly fully coalescing, it is clear that its characteristic time of coalescence has to be

lower than 15 seconds (as it manages to coalesce even in this case). On the other

side as the 50%MMA is only partially coalescing even at =1x10-5, its characteristic

time of coalescence has to be higher than 45 seconds.

A physical evidence to these assumed values can be provided by evaluating the

particles viscosities. Due to the proportional nature of equation (1.36) this can be

carried out only with a magnitude order magnitude approach, assuming for simplicity

equation (1.36) as strict equality and a fixed particles surface tension (for PMMA

22.69 [mN/m] [19]). Postulating for the 30%MMA and 50%MMA samples as

characteristic times of coalescence respectively 1-15 [s] and 60-120 [s], the

corresponding particles viscosities result 1.13x105-1.7x106 [Pa s] and 6.8x106-

1.36x107 [Pa s]. Since the obtained viscosities are consistent with typical values

reported in the literature [20], the coalescence characteristic times might actually lie

around the suggested values.

4.1.1.2 Characterization at high volume fractions:

In order to investigate the gelation of the particles, salt-induced aggregation kinetics

were carried out in DLCA conditions at high latexes volume fractions (0.05-0.1) for all

the samples. At high particles concentrations aggregation becomes the most

dominant phenomenon ( coal agg ) and typically ends up in gels formations. In our

particular conditions the characteristic times of aggregation agg (evaluated through

equation (4.1)) are as expected very small (in the range 9x10-3-4x10-3 [s]). It is

therefore reasonable to neglect coalescence in these experiments, as for the

particles characteristic times to be so small, the particles should have viscosities in

the order of 9x102-2x103 [Pa s].

Experimentally 3 [ml] of 5 [M] NaCl solution were poured into 3 [ml] of the high DC

purified latexes at 25 [ºC]. Depending on how the salt solution was poured into the

57

latexes two results were obtained: if the salt solution was slowly poured into the

latexes leaving it diffusing through, gel formation occurred for all the samples; if the

salt solution was rapidly poured into the latexes, gel formation occurred for the

30%MMA and 50%MMA samples but not for the 60%MMA and 70%MMA ones for

which only large aggregates were found. Furthermore, once formed, these 60%MMA

and 70%MMA gels were very weak and if mildly agitated showed to break. The

broken gel aggregates were diluted and measured in the SLS; fd 2.5 were found,

meaning that the clusters were rearranging in more compact structures. On the other

hand the 50%MMA and 30%MMA gels proved to be very compact regardless the

pouring method used.

Since at 25 [ºC] the 30%MMA and 50%MMA particles are both above their respective

gT (cf. Table 2-5)coalescence can occur. In these conditions the 30%MMA and

50%MMA particles behave slightly viscously and, when aggregation is induced, can

partially interpenetrate with one another, sticking and forming resistant aggregates.

On the contrary the 60%MMA and 70%MMA particles at 25 [ºC] are both below their

respective gT (cf. Table 2-5), coalescence cannot occur and at the minimum stress

the aggregates undergo breakage.

Therefore, in spite of the fact that at high volume fraction coal agg , the role of

coalescence is very important as it affects the gel strength/weakness (particularly

note that this fact has to be carefully considered when studying the gelation of the

particles in shear).

As additional experiment, the 60% MMA high DC sample was heated up to 45 [ºC]

(60%MMA gT 35 [ºC]) and the 5 [M] NaCl solution was rapidly poured into the latex.

In these conditions a strong gel was formed and maintained its structure also when

the sample was cooled to room temperature.

58

4.1.2 RLCA

Before investigating shear conditions it was required to elucidate how our particles

basically behave when there is no imposition of an external velocity field but repulsive

interactions are present (stagnant RLCA).

Assuming our particles undergoing DLVO interactions, at first it will be discussed how

the van der Waals and the electrostatic forces affect our samples potential energy

barrier, then the effect of the electrostatic forces on the samples stability will be

clarified.

Several analytical solutions for Van der Waals interaction potential energies are

available in the literature [10]; in general they always take the form

( )AV A f geometry ,where A is the Hamaker constant. The value of A , 1.05x10-20

[J] for PMMA dispersions in water [10], does not depend on the samples composition.

This can be estimated through the Lifshitz theory of macroscopic Van der Waals

interaction in the simplest case of slabs of two identical material 2 interacting across

a medium 1 [10, 21] (McLachlan equation):

22 2 2

2 1 2 1

2 2 2

2 1 2 1

3 ( )3

4 ( )32 2

Bk T n nhA

n n

(4.7)

Where i are the static dieletric constant, in the refractive indices in the visible range,

h is the Planck constant and is the UV peak absorption frequency.

Since our PMMA samples dielectric constants, refractive indexes and UV peak

absorption frequencies in equation (4.7) are similar, the value of A can be assumed

as composition independent. The geometry is given by the one of the interacting

system and for each of our samples results the same (sphere).

Therefore since both the geometry and Hamaker constant do not differ changing the

samples compositions, the Van der Waals interactions affect our samples interaction

potentials energies in the same way.

On the other side the impact of the electrostatics on our samples energetic barriers

can be directly experimentally evaluated. This was carried out by particle surface

charges (cf. Figure 4-10) and ζ-potential (cf. Figure 4-11) measurements.

59

Figure 4-10 Absolute values of the surface charge density as function of the %MMA

Figure 4-11 ζ-Potential at 25 [ºC] as function of the %MMA measured at 1x10-5

with

10 [mM] NaCl ( light blue) and 140 [mM] NaCl (dark blue). Increasing the salt

concentration leads to a lower absolute value of the potential .

60

From Figure 4-10 can be observed that the samples exhibit different surface charges

densities; more in detail the trend seems to be the higher the BA%, the higher the

surface charge density; such a behavior can be explained as the effect of different

hydrophobicity-hydrophilicity values for the MMA and BA (the solubility at 20 [ºC] in

water are respectively 16 [g/L] and 2 [g/L] [22] [23]). During the polymerization, which

involves a homogenous nucleation mechanism, growing oligoradicals chains are

formed; the length at which these chains precipitate on the particles nuclei is given by

their solubility in water: the lower it is, the sooner they will precipitate. If long chains

are formed the KPS, which is attached at one of the end, will remain wrapped inside

and lower surface charges are found. Since according to the solubility the MMA

forms longer chains than the BA, less charged groups are expected to be found for

the rich %MMA samples.

The surface charges differently affect the total interaction potential energies shapes.

In particular, the larger they are, the more the particles repel each other and therefore

the higher the absolute maxima values mV .

This can be further appreciated by measuring the samples ζ-potential. The ζ-potential

values reported in Figure 4-11 result different from one sample to the other and follow

the same trend of the corresponding surface charges (cf. with Figure 4-12). Note that

experimentally ζ-potential measurements have to be performed at very low salt

concentrations (10 [mM]). The higher salt concentration (140 [mM]) was tested since

comparable ones were employed in shear conditions. As expected increasing the salt

concentration leads to a lower absolute value of the potential but only slightly affects

the trend between the samples which remains in the experimental error similar.

In general higher absolute values of potential energy barriers result in higher stability.

The samples stability was determined by measuring the samples critical coagulation

concentration (cf. Figure 4-13) and by calculating the corresponding Fuchs stability

ratios (cf. Figure 4-14).

Several aggregation kinetics (reported in APPENDIX III) were run in the DLS at 25

[ºC] with 1x10-5 starting from high NaCl concentrations which were progressively

decreased. In DLCA where W =1 the rate of aggregation is the fastest and all the

aggregation kinetics overlap; as soon as the RLCA regime is entered the aggregation

kinetics are slower and do not overlap any more with the DLCA ones.

61

Figure 4-13 Values of the crit ical coagulation concentration as function of the MMA%

measured at 1x10-5

and 25 [ºC]

Figure 4-14 Values of the Fuchs stabil ity ratio as function of the NaCl concentration

and MMA% at 1x10- 5

and 25 [ºC]

62

The CCC was determined as the lowest salt concentration at which the aggregation

curves were found to be overlapped.

The Fuchs stability ratios were evaluated by fitting the aggregation curves according

to the mathematical model and numerical methods described in [24], [14], [25], [26].

If the electrostatic contributes (Figure 4-10 and Figure 4-11) are compared with the

overall potential ones (Figure 4-13 and Figure 4-14), similar trends can be observed.

Nevertheless as shown in Figure 4-13 and Figure 4-14 increasing the %MMA content

from 60% to 70% reveals a catastrophic loss in stability for the MMA rich samples.

This loss of stability cannot be explained only in terms of electrostatics since the

respective surface charges and ζ-potential values are comparable for all the samples,

and might be ascribed to a material effect or a non-DLVO contribution (cf. [10]).

63

4.2 Shear Aggregation

At last, once the behaviors of our samples were clarified in stagnant, the interplay

between coalescence and aggregation was investigated in shear conditions.

In order to discuss our results, it is necessary to understand the shear induced

aggregation mechanism; this can be done by introducing the characteristic time of

aggregation in shear, which by combining equation (1.32) with equation (1.34)

results:

362

0

m

B B

mV V aPe

k T k T

agg DLCA

We e

N

(4.8)

If shear is introduced into the system the characteristic time of aggregation depends

on the competition between the interaction potential and the shear destabilizing

effect.

To better explain the physical meaning of equation (4.8) it is possible to plot the

aggregation rate constant as a function of the Peclet (Pe) number (cf. Figure 4-15).

Figure 4-15 shows that two limit regimes are possible: at low Peclet numbers Pe<<1

Figure 4-15Normalized aggregation rate constants between two particles as a function

of Peclet number. In the left frame the rate of doublet formation is reported at four

levels of particles surface potential. In the r ight frame the rate of doublet formation is

reported at a f ixed surface potential but at different ionic strength ( increasing toward

bottom). Left and right pictures taken respectively from [27] and [6].

64

the system is in purely Brownian-like conditions and the aggregation rate is

dominated by the value of the repulsive energy barrier mV (RLCA); in these situations

the exponential term of equation (4.8) is positive and large characteristic aggregation

times result; at high Peclet numbers Pe>>1 the system is in purely shear induced

regime and the aggregation rate results practically independent from the value of the

repulsive energy barrier mV (RLCA); in these conditions the exponential term of

equation (4.8) is negative and small characteristic aggregation times result.

Furthermore, if the system starts at low Pe, as soon as aggregation takes place the

Peclet number increases rapidly with the cluster sizes Pe3a and the pure shear

induced region is entered. The exponential term of equation (4.8) becomes in fact

negative and the characteristic times of aggregation drop abruptly.

The theory forecasts therefore an initial induction time followed by an explosive rise

of viscosity typically observed in colloidal system under shear (i.e. gelation).

This system behavior can be better appreciated looking at the relation between the

volume fraction and the medium viscosity, which can be expressed for non-diluted

solutions by the Krieger-Dougherty equation [28]:

[ ]

0

1

max

max

(4.9)

Where 0 is the viscosity at 0 , [ ] is the intrinsic viscosity and max is the packing

fraction, its upper limit is approximately 0.64 for random close packaging and roughly

0.71 for the closest possible arrangements of spheres. Using the geometric series

and expanding the right member of equation (4.9) leads to a power dependence of

the medium viscosity. If the system is aggregating at low Pe, since the aggregates

volume is increasing slowly, remains almost constant (cf. equation (1.35)) and a

flat medium viscosity profile results (initial induction time). As soon as larger

aggregates are formed, the aggregates volume and rapidly grow in time due to the

exponential increase of Pe, the medium viscosity therefore according with equation

(4.9) explodes until at last the limit where a gel is formed is reached.

On the other hand if the aggregating particles undergo coalescence the characteristic

time of aggregation will be affected as the cluster size will be shrinked by the on-

going coalescence, therefore reducing the increase in terms of Pe number, slowing

65

down the aggregation process. If full coalescence is possible( coal agg ) no occupied

volume growth would be allowed, the volume fraction and the viscosity would remain

constant and so no gel could be formed; if coalescence occurs partially, gel could be

formed but longer initial induction times and as consequence delayed gelation times

would be observed.

Several shear-induced aggregations were carried out in the rheometer for the

samples 30%MMA, 50%MMA and 60%MMA (cf. Figure 4-16 - Figure 4-24).

Only these samples were sheared because it was impossible to raise the rheometer

temperature over 55 [ºC], due to problems related with the evaporation of the latexes,

and as previously discussed the 70%MMA sample showed to be very sensitive to

breakage already in stagnant condition when the experimental temperature was

below its gT . The analysis were performed at a fixed shear rate 4900 [Hz] and

final DC=5%. In order to enhance samples coalescence, according to the samples

gT values listed in Table 2-5, three different temperatures (25 [ºC], 35 [ºC], 45 [ºC])

were analyzed. Furthermore in order to observe shear induced aggregations in

reasonable experimental times but still remaining in RLCA regime it was necessary to

reduce the repulsive effect of the energy barrier maximum mV by adding small

quantities of salt. In particular, three different NaCl concentrations 120 [mM], 130

[mM] and 140 [mM] were identified as the proper ones. The results are reported in

Figure 4-16 - Figure 4-24. In these graphs is shown the time evolution of the samples

viscosity at the different temperatures and salt concentrations tested; it can be seen

that gelation occurs for the majority of the samples (the viscosity abruptly increases

after a given lag time).

66

Figure 4-16 Evolution of viscosity as funct ion of time in the rheometer for 30%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

25 º[C].

Figure 4-17 Evolution of viscosity as funct ion of time in the rheometer for 30%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

35 º[C].

67

Figure 4-18 Evolution of viscosity as funct ion of time in the rheometer for 30%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

45 º[C].

Figure 4-19 Evolution of viscosity as funct ion of time in the rheometer for 50%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

25 º[C].

68

Figure 4-20 Evolution of viscosity as funct ion of time in the rheometer for 50%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

35 º[C].

Figure 4-21 Evolution of viscosity as funct ion of time in the rheometer for 50%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

45 º[C].

69

Figure 4-22 Evolution of viscosity as funct ion of time in the rheometer for 60%MMA;

140 [mM]NaCl at 25 º[C].

Figure 4-23 Evolution of viscosity as funct ion of time in the rheometer for 60%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

35 º[C].

70

Figure 4-24 Evolution of viscosity as funct ion of time in the rheometer for 60%MMA;

Different salt concentrations (140 [mM], 130 [mM] and 120 [mM])of NaCl are reported at

45 º[C].

At these experimental conditions the initial Peclet number values are in the range 10-

11. As previously discussed if the initial Peclet values exceed a certain threshold, the

doublet formation rate becomes interaction potential independent and only

dominated by the shear induced aggregation. As a main consequence, if our

samples would be located in that region, each of them would gel at the same time

regardless of the salt amount present. As shown in Figure 4-16 - Figure 4-24, this

does not happen in our cases, indicating that our samples are not in pure shear-

conditions and their aggregation rate is indeed affected by their potential. In this

frame, the aggregation and coalescence characteristic times depend on the samples

salt concentrations, temperatures and compositions. Each of these contributions will

be individually discussed in the following sections.

4.2.1 Salt effect

From Figure 4-16 - Figure 4-24 the effect of the salt on the characteristic time of

aggregation can be clearly appreciated: the higher is the salt concentration the

71

sooner the gelation occurs. This trend is explainable in terms of double layer

compression as can be seen looking at the form of the total interaction potential

energy which in the simplest but sufficient case of two slabs at distance r with small

overlapping is given by [1]:

2

0264 exp

12tot B

A rV N k TZ

r

`(4.10)

Where 0Z tanh4 B

ze

k T

and 0 is the surface potential. The first and second terms on

the right hand side of equation (4.10) describe respectively Van der Waals and

electrostatics interactions. If the salt concentration increases, the Van der Waals

contribute (salt independent) remains unchanged where as the Debye length

decreases according to equation (1.9); if decreases results from equation (4.10) a

lower electrostatic repulsive contribute to totV , in particular to the maximum value.

From equation (4.8) if the repulsive term of mV is progressively reduced, smaller

characteristic aggregation times are obtained.

This situation is depicted in the right frame of Figure 4-15 where the rates of doublet

formation, reported at a fixed surface potential and at different ionic strength, exhibit

a step shape in the RLCA region, in detail the higher is the ionic strength, the higher

is the aggregation rate and the lower is the gel time once the shear induced region is

entered.

4.2.2 Temperature effect

In Figure 4-25 - Figure 4-27 the temperature impact for each sample composition is

reported. As values of gelt were taken the intersections between two linear

regression, one made with the last medium viscosity measures and the other with the

starting ones of Figure 4-16 - Figure 4-24.

72

Figure 4-25 Gel t imes for 30% MMA as function of temperature and salt concentration

Figure 4-26 Gel t imes for 50% MMA as function of temperature and salt concentration

73

Figure 4-27 Gel t imes for 60% MMA as function of temperature and salt concentration

Figure 4-26 and Figure 4-27 show that increasing the temperature leads to

progressively lower gelation times for the 50%MMA and 60%MMA samples. On the

other hand the 30% MMA sample (Figure 4-25) shows a peculiar trend: upon

temperature increase, the gel times initially increase (compare 25 [oC] and 35 [oC])

while a further increase (from 35 [oC] to 45 [oC]) leads to a further reduction of the gel

times.

The expected effect of a temperature increase on the gel time is a delay in the

gelation due to an enhancement of coalescence as more compact clusters with a

smaller occupied volume fraction are formed. The results reported show that this

occurs only in case of the 30%MMA sample at 35 [ºC] while in all the other

experiments the gelation occurs sooner the higher the temperature. This trend can be

explained in terms of effects competition between aggregation and coalescence

times. In fact if the temperature increases the medium and particles viscosities

decrease and, according to equations (1.36) and (4.8), the coalescence and

aggregation characteristic times are respectively shorter and longer. On the other

hand as the temperature increases a destabilizing effect takes place (the presence

and nature of this destabilizing effect and its temperature dependence will be further

unveiled) and affects the characteristic times of aggregation which result

74

progressively shorter. In the explored temperature range the destabilizing effect

increases significantly with the temperature and always overcomes the coalescence

ones. There is an exception for the points at 35 [ºC] of the 30%MMA: since for this

sample coalescence occurs the most, its contributions at 35 [ºC] dominate the

destabilizing ones leading therefore to a delay in the gel time; at 45 [ºC] nevertheless

destabilization, which increases in temperature, dominates again and the delay effect

of coalescence disappears.

The presence of a destabilizing effect that takes places as the temperature increases

was proven by CCC measurements. (cf. Figure 4-28). The 30%MMA, 50%MMA and

60%MMA samples CCC were in fact measured again at 45 [ºC] in the same

conditions as they were measured at 25 [ºC];as shown, increasing the temperature

leads to a decrease in the CCC.

Figure 4-28 Comparison of the crit ical coagulation concentration values as function of

the MMA% measured at 1x10-5

and T 25, 45 [ºC]

Since the samples stabilities, as previously discussed, are related to the absolute

values of the potential energy barriers, the nature of this temperature behavior can

be extrapolated by looking at the relative dependence of the DLVO interaction

potential (equation (4.10)). In detail the impact of the temperature on the DLVO

75

potential attractive term can be appreciated by substituting equation (4.7) in

equations (4.10) and (4.8); as can be seen only the second member of the Hamaker

constant slightly decreases if the temperature increases. Weaker Van der Waals

contributes would result in higher repulsive contributes in the DLVO potential and in

particular for the energetic barrier maximum. As a consequence a longer aggregation

characteristic time should be expected. Thus this effect is insignificant since it would

lead to the opposite trend compared with the one observed. The impact of the

temperature on the DLVO potential repulsive term can be appreciated by substituting

equation (4.10) in equation (4.8); as can be seen the factor Bk T in the electrostatic

term cancels out and only a square root temperature dependence results in the

Debye length. This dependence in the range of temperatures investigated is

negligible (3%) and therefore the electrostatic contributes to the DLVO potential can

be practically considered temperature independent. Furthermore as additional

evidence for the electrostatics temperature independence the ζ-potential values were

measured at 45 [ºC] (cf. Figure 4-29).

Figure 4-29 Comparison between ζ-potential values measured at 10 and 140 [mM] with

1x10-5

and T 25, 45 [ºC]

76

As can be seen from they do not differ much from the ones at 25 [ºC].

Since the stability decrease upon temperature increase cannot be explained in terms

of DLVO potential which has been substantially proven as temperature independent,

the nature of this destabilizing effect must be ascribed to non DLVO contributions.

These contributions can be condensed in a term which, if introduced into the

expression of the DLVO potential (equation (4.10)), decreases the overall maximum

value of the energetic barrier. From equation (4.8) as the values of the overall

energetic barrier are reduced, smaller characteristic times of aggregation result

4.2.3 Composition effect

In order to elucidate the impact of the sample composition on the characteristic times

of coalescence are reported in Figure 4-30 - Figure 4-32 the gelation times of all the

samples as function of the salt concentrations at each specific temperature tested.

Figure 4-30 Gel t imes for 30%MMA, 50%MMA, 60% MMA as function of composition

and salt concentration at 25 [ºC]

77

Figure 4-31 Gel t imes for 30%MMA, 50%MMA, 60% MMA as function of composition

and salt concentration at 35 [ºC]

Figure 4-32 Gel t imes for 30%MMA, 50%MMA, 60% MMA as function of composition

and salt concentration at 45 [ºC]

78

These graphs show that the 30%MMA and 50%MMA samples exhibit progressively

shorter gelation times at all the temperatures experimented. On the other side the

60%MMA sample gelt values are always placed in the middle of the previous two.

Furthermore it is worth to point out that at 25°[C] for this sample no gelation was

reported in the experimental time.

The expected effect of increasing the BA content is to observe longer gelations as

the resulting polymers have smaller gT and hence an increased coalescence. This

trend is observed only for the 30%MMA and the 50%MMA samples.

In order to explain the results of the 60%MMA sample it is worth to remark that if the

sample is tested below its gT , it is strongly subjected to breakage; furthermore

breakage is strongly reduced as coalescence takes place. As consequence around

the gT the competition between these two phenomena have to be considered in

order to figure out our sample behavior. At 25 [°C] the 60%MMA sample is below its

gT (35°[C]) and coalescence cannot occur. Breakage is the dominating phenomenon

and therefore no gel can be formed. At 35 [°C] despite the 60%MMA sample it is

starting to coalesce, the particles are not interpenetrating enough in order to avoid

breakage and longer gelation times than the 50%MMA sample result. At 45°[C]

coalescence occurs more than at 35 [°C] (compare 60%MMA sample gelt in Figure

4-31 and Figure 4-32) but still the particles bond are weak and again as

consequence of breakage longer gelation times than the 50%MMA sample result.

As shown in Figure 4-30 - Figure 4-32 for the 30%MMA and 50%MMA samples the

effect of breakage results completely negligible and increasing the BA content

reduces progressively the characteristic times of coalescence.

The reason for which only for the 60%MMA breakage is observable is due to the

different coalescence between the samples. As previously discussed, the material

glass transition does not occur at a specific temperature but in region centered

around it. As can be seen from the plot listed in APPENDIX I at 25 [°C] the 30%MMA

and 50%MMA samples are already above their respective glass transition. This is not

the case for the 60%MMA sample where at 35 [°C] and 45 [°C] it is still in progress.

As consequence for this sample at the temperatures tested coalescence occurs less

compared with the 30%MMA and 50%MMA samples and therefore the competition

aggregation – breakage is observable.

79

5 CONCLUSION:

The scope of the present work was to study the interplay between coalescence and

aggregation under shear for polymeric colloidal dispersions.

Four latexes of poly(methylmethacrylate-co-butylacrylate) (PMMA-co-BA) have been

synthesized by starved emulsion polymerization in a semi-batch reactor. The different

ratios of methyl methacrylate and butyl acrylate employed allowed preparing particles

exhibiting a glass transition temperature gradient which allowed studying the

behavior of coalescence in the system.

Initially the interplay aggregation-coalescence in stagnant conditions (DLCA) was

explored. Since coalescence can occur only above the glass transition temperature,

aggregations induced by salt (NaCl) were performed at different temperatures.

Furthermore in order to clearly unveil the effects of coalescence these salt induced

aggregations were carried out at low and high latexes volume fractions. At low

volume fraction, since the characteristic time of coalescence is smaller than the

aggregation one, it is found that coalescence affects aggregation resulting in lower

aggregates gyration radii compared with the non coalescing ones and in high fractal

dimension. Faster coalescence in general occurs the higher is the value of the

sample temperature over its gT until eventually a maximum coalescence rate is

reached. The reason is due to the particles viscosity which plays a crucial role in the

characteristic time of coalescence: as the temperature rises, viscosity decreases

increasing the rate of coalescence. As consequence it resulted that the rich BA

samples were progressively coalescing more the higher was the BA content. At high

volume fractions, since the characteristic time of coalescence is larger than the

aggregation one, all the samples destabilized with salt ended up in gels; in these

conditions it is found that coalescence affects aggregation through the gels strength:

the samples, if their experimental temperature was below their corresponding gT ,

formed weak gels (gels that, if mildly agitated, showed to break rearranging in more

compact structures); on the other side if their experimental temperature was above

their corresponding gT ,strong gels were formed (gels that, if shaken, did not show

80

any sign of breakage). The gel strength is explainable in terms of coalescence that

allows the particles to partially interpenetrate one with another, sticking and forming

resistant aggregates.

Successively the particles aggregation in RLCA was investigated. In these conditions

it was found that the Van der Waals contributes to the samples mV values are

composition independent. The electrostatic impact on mV values was evaluated for

each sample by surface charges and ζ-potential measurements. It results in general

that increasing the BA content slightly increases the surface charges, the ζ-potential

and as consequence the mV values. Higher absolute values of potential energy

barriers lead to higher stability. The samples stability was determined by measuring

their critical coagulation concentrations and is found to follow the same trend of the

mV values. In spite of that increasing the MMA content over a certain threshold

reduces dramatically the rich MMA samples stability. Since the surface charges and

ζ-potential values are comparable for all the samples, this behavior is ascribed to a

material effect or a non-DLVO contribution.

Furthermore as the samples stability was measured at higher temperature it resulted

to drop abruptly. This remarkable destabilizing effect due to the temperature cannot

be explained in terms of DLVO potential which is substantially temperature

independent and is due to non DLVO contributions.

Finally the interplay between aggregation and coalescence was investigated in shear

conditions. Shear induced aggregation were performed at different salt

concentrations and temperatures at a fixed dry content and shear rate.

In these conditions where the initial samples aggregation rate is dominated by the

value of the repulsive energy barrier, it is found that the competition between

aggregation and coalescence depends on the samples salt concentrations,

temperatures and compositions.

Increasing the salt concentration reduces only the characteristic times of aggregation

(double layer compression).

If the temperature increases two competitive effects take place: on one hand the

coalescence and aggregation characteristic times result respectively shorter and

longer as the medium and particles viscosities decrease. On the other hand the

81

thermal non-DLVO destabilizing effect decreases the characteristic times of

aggregation. In the explored temperature range these destabilization contributions

increase significantly with the temperature and in the majority of the cases overcome

the coalescence effects. As consequence the impact of the temperature is relevant

only for the characteristic time of aggregation.

As exception, the reduction of the characteristic time of coalescence due to effect of

the temperature was appreciated for the most coalescing sample where coalescence

becomes comparable with aggregation; in this case in fact upon temperature

increase, the gel times initially increase while a further increase leads to a further

reduction of them.

Increasing the BA content reduces progressively the characteristic times of

coalescence. This tendency is confirmed only if the sample is above its glass

transition. If the sample is tested below its glass transition it results strongly subjected

to breakage which prevents gel formations. During the glass transition it is possible to

observe the interplay between coalescence and breakage. As coalescence takes

place, breakage is considerably reduced until over a certain point it becomes

negligible and longer gelation times are found as the resulting polymers have an

increased coalescence.

82

References

1. Morbidelli, Polymer Reaction & Colloid Engineering LECTURE NOTES, 2013. 2. Nomura, M., H. Tobita, and K. Suzuki, Emulsion polymerization: Kinetic and

mechanistic aspects. Polymer Particles, 2005. 175: p. 1-128. 3. Jose´ C. de la Cal, J.R.L., Jose M. Asua, Alessandro Butte`, Giuseppe Storti,

and Massimo Morbidelli, Handbook of Polymer Reaction Engineering. p. Chapter 6, Emulsion Polymerization.

4. Waychunas, G.A., Structure, aggregation and characterization of nanoparticles. Nanoparticles and the Environment, 2001. 44: p. 105-166.

5. M. Elimelech, J.G., X. Jia, R.A. Williams, John Gregory, Xiaodong Jia and Richard A Williams, Particle Deposition & Aggregation.

6. Zaccone, A., et al., Theory of activated-rate processes under shear with application to shear-induced aggregation of colloids. Physical Review E, 2009. 80(5).

7. Frenkel, J., Viscous flow of crystalline bodies under the action of surface tension. Journal of Physics, 1945. IX.

8. R. M. Wheaton, L.J.L., DOWEX Ion Exchange Resins Fundamentals of Ion Exchange, 2000, Dow Liquid Separations Office.

9. Dietrich Braun , H.C., Matthias Rehahn, Helmut Ritter, Brigitte Voit, Polymer Synthesis: Theory and Practice Fundamentals, Methods, Experiments. 2012: Springer.

10. Berg, J.C., An introduction to Interfaces & Colloids, The Bridge to Nanoscience. 2010: World Scientific Publishing Co. Pte. Ltd.

11. Sorensen, C.M., Light scattering by fractal aggregates: A review. Aerosol Science and Technology, 2001. 35(2): p. 648-687.

12. Macosko, C.W., Rheology: Principles, Measurements, and Applications. 1994: WILEY-VCH.

13. Sandkühler, P., Kinetics of Aggregation and Gel Formation in Colloidal Dispersions, 2004.

14. Lattuada, M., et al., Aggregation kinetics of polymer colloids in reaction limited regime: experiments and simulations. Advances in Colloid and Interface Science, 2003. 103(1): p. 33-56.

15. Wu, H., M. Lattuada, and M. Morbidelli, Dependence of fractal dimension of DLCA clusters on size of primary particles. Advances in Colloid and Interface Science, 2013. 195: p. 41-49.

16. Xie, D.L., et al., Criticality for shear-induced gelation of charge-stabilized colloids. Soft Matter, 2010. 6(12): p. 2692-2698.

17. Ehrl, L., M. Soos, and M. Morbidelli, Dependence of aggregate strength, structure, and light scattering properties on primary particle size under turbulent conditions in stirred tank. Langmuir, 2008. 24(7): p. 3070-3081.

18. Eggersdorfer, M.L., et al., Multiparticle Sintering Dynamics: From Fractal-Like Aggregates to Compact Structures. Langmuir, 2011. 27(10): p. 6358-6367.

19. Wypych, G., Handbook of Polymer. 2013. 20. Nijenhuis, D.W.V.K.a.K.T., Properties of Polymers. Fourth Edition ed. 21. Israelachvili, J.N., Intermolecular and Surface Forces, Third edition. 2011. 22. METHYL METHACRYLATE CAS N°: 80-62-5, U. Chemicals, Editor. 23. N-BUTYL ACRYLATE CAS N°: 141-32-2, U. Chemicals, Editor.

83

24. Lattuada, M., et al., Modelling of aggregation kinetics of colloidal systems and its validation by light scattering measurements. Chemical Engineering Science, 2004. 59(8-9): p. 1783-1798.

25. Kumar, S. and D. Ramkrishna, On the solution of population balance equations by discretization .1. A fixed pivot technique. Chemical Engineering Science, 1996. 51(8): p. 1311-1332.

26. Kumar, S. and D. Ramkrishna, On the solution of population balance equations by discretization .2. A moving pivot technique. Chemical Engineering Science, 1996. 51(8): p. 1333-1342.

27. Wu, H., et al., Effect of Temperature on High Shear-Induced Gelation of Charge-Stabilized Colloids without Adding Electrolytes. Langmuir, 2010. 26(4): p. 2761-2768.

28. Principles of Colloid and Surface Chemistry, Third Edition, Revised and Expanded. 1997.

84

APPENDIX I

Figure 1 Heat f lux as function of temperature for 70%MMA

Figure 2 Heat f lux as function of temperature for 60%MMA

85

Figure 3 Heat f lux as function of temperature for 50%MMA

Figure 4 Heat f lux as function of temperature for 30%MMA

86

APPENDIX II

Figure 1 0I vs. gR plot for30%MMA in the small angle static l ight scattering at

1x10-5

Figure 2 0I vs. gR plot for50%MMA in the small angle static l ight scattering at

1x10-5

87

Figure 3 0I vs. gR plot for60%MMA in the small angle static l ight scattering at

1x10-5

Figure 4 0I vs. gR plot for70%MMA in the small angle static l ight scattering at

1x10-5

88

Figure 5 0I vs. gR plot for30%MMA in the small angle static l ight scattering at

2x10-5

Figure 6 0I vs. gR plot for50%MMA in the small angle static l ight scattering at

2x10-5

89

Figure 7 0I vs. gR plot for60%MMA in the small angle static l ight scattering at

2x10-5

Figure 8 0I vs. gR plot for 70%MMA in the small angle static l ight scattering at

2x10-5

90

Figure 9 0I vs. gR plot for 30%MMA in the small angle static l ight scattering at

3x10-5

Figure 10 0I vs. gR plot for 50%MMA in the small angle static l ight scattering at

3x10-5

91

Figure 11 0I vs. gR plot for 60%MMA in the small angle static l ight scattering at

3x10-5

Figure 12 0I vs. gR plot for 70%MMA in the small angle static l ight scattering at

3x10-5

92

APPENDIX III

Figure 1 Aggregation kinetics in the dynamic light scattering at 1x10-5

and T 25

[ºC] for 30%MMA

Figure2 Aggregation kinetics in the dynamic light scattering at 1x10-5

and T 25

[ºC] for 50%MMA

93

Figure 3 Aggregation kinetics in the dynamic light scattering at 1x10-5

and T 25

[ºC] for 60%MMA

Figure 4 Aggregation kinetics in the dynamic light scattering at 1x10-5

and T 25

[ºC] for 70%MMA

94

Figure 5 Aggregation kinetics in the dynamic light scattering at 1x10-5

and T 25

[ºC] for 100%MMA

Recommended